Degree Thesis Flexural Rigidity (D) in Beams. Author: Zious Karis. Instructor: Rene Herrmann


 Amber Marsh
 1 years ago
 Views:
Transcription
1 Degree Thesis Flexural Rigidity (D) in Beams Author: Zious Karis Instructor: Rene Herrmann Degree Thesis Materials Processing Technology 2017
2 DEGREE THESIS Arcada University of Applied Sciences, Helsinki, Finland Degree Programme: Identification number: Author: Title: Supervisor (Arcada): Materials Processing Technology Zious Karis Flexural Rigidity in Beams Rene Herrmann Commissioned by: Abstract: This thesis presents the theory behind the symmetrical and unsymmetrical beams with different crosssections, the mathematical procedure in calculating the flexural rigidity of symmetrical beams and summarizing the experimental verification by mathematical data processing of the flexural rigidity by threepoint bending. The core of the method section is to test theoretically by using the composite compressive strength modeler (CCSM) software and experimentally in the laboratory by using the material bending machine a solid fiberglass and a sandwich beam. The results obtained for the solid fiberglass was found to be theoretically 32 Nmm 2 and experimentally 31.1 MNmm 2. For the sandwich beam along the direction of the orientation of the fiber theoretically 155 Nmm 2 and experimentally Nmm 2. As for the sandwich beam with the same properties but with a direction perpendicular to the fiber theoretically 45.1 Nmm 2 and experimentally Nmm 2. The comparison of flexural rigidity values was found to be 3.1% for the solid fiberglass, 1.1% for the sandwich beam along the direction of the orientation of the fiber and 4.6% with a direction perpendicular to the fiber. Moreover, for the foursection module, the values obtained for the moments of the outer layer contributed seven times more to rigidity than the inner layer and for the sixsection module the second outermost layer contributed seven times more than the innermost layer and the outermost layer nineteen times more to rigidity than the innermost layer. Keywords: Flexural rigidity, deflection in beams, symmetrical bending, sandwich structure, composite beams, (CCSM) modeler, threepoint bending Number of pages: 60 Language: English Date of acceptance: 2
3 CONTENTS 1 INTRODUCTION Problem Definition Aims and Objectives Method Background Flexural Rigidity THEORY Second Moment of Area Materials Composite Materials Composites versus Metallic Bending Stiffness of Beams Theory of Simple Bending with Assumptions Made Bending of Composite Beams Symmetrical Bending Examples of Symmetrical Bending Unsymmetrical Bending History of Sandwich Structure Sandwich Structure Flexural Rigidity in Sandwich Beams Deflection of Beams METHOD Composite Compressive Strength Modeler (CCSM) A Solid UD Lamina Bending ThreePoint & FourPoint Bending RESULTS Bending Test and CCSM Modelling DISCUSSION
4 6 CONCLUSION REFERENCES
5 Figures Figure 2.1 Composite structure [6] Figure 2.2 Steel vs. sandwich [9] Figure 2.3 Strain [11] Figure 2.4 Ibeam [13] Figure 2.5 Rectangular crosssection Figure 2.6 Centroidal xaxis Figure 2.7 Twosections Figure 2.8 Foursections Figure 2.9 Sixsections Figure 2.10 Rectangular beam [15] & Figure 2.11 Upward restoring force [15] Figure 2.12 Tbeam [16] Figure 2.13 Efficiency of sandwich structure [9, p. 256] Figure 2.14 Sandwich structure [18, p. 5] Figure 2.15 Sandwich beam cross section [4] Figure 2.16 Deflection and curvature due to bending [20] Figure 2.17 Cantilever beam [20] Figure 2.18 Simply supported beam [20] Figure 2.19 Simply supported beam, deflection at center Figure 2.20 Simply supported beam, uniformly distributed load Figure 3.1 Principal material axes in a UD lamina [23] Figure 4.1 Materials testing machine Figure 4.2 Solid fiberglass  theoretical Figure 4.3 Solid fiberglass theoretical d Figure 4.4 Solid fiberglass  experimental Figure 4.5 Sandwich beam 1  theoretical Figure 4.6 Sandwich beam 1 theoretical d Figure 4.7 Sandwich beam 1  experimental Figure 4.8 Sandwich beam 2  theoretical Figure 4.9 Sandwich beam 2 theoretical d Figure 4.10 Sandwich beam 2  experimental
6 Tables Table 1. Composites versus metals under certain conditions. [9] Table 2. ASTM standards for threepoint bend. [27] Table 3. ASTM standards for fourpoint bend. [27] Table 4. Values for the CCSM Modeler Table 5. Results
7 List of Symbols Name Symbol Unit 1. Flexural rigidity D Nm 2 2. Bending modulus (material property) E Pa = N/m 2 3. Young s modulus of faces Ef Pa 4. Second moment of inertia I m 4 5. Width b m 6. Thickness t m 7. Distance d m 8. Force F N 9. Height h m 10. Moment/Bending moment M Nm 11. Stress σ Pa = N/m Length L m 13. Area A m Strain Ε  or mm/mm 15. Shear stress Q Pa 16. Slope Θ (k) N/mm 17. Distance along beam x m 18. Radius of neutal axis r m 19. Distance of surface (NS) y m 20. Torque τ Nm 21. Deflection Y mm 22. Distributed load W N/m 7
8 FOREWORD I would like to thank Mr. Rene Herrmann for the supervision throughout this thesis. I would like to thank all the professors and staff for their guidance during my three years of studying at Arcada University of Applied Sciences. Special thanks to Mr. Erland Nyroth for his encouragement and advices throughout my studies. Finally, I would like to thank my family and friends for their continued support over last few years, particularly during the completion of this thesis. Special thanks to my father for his unlimited support and encouragement. Special thanks also to Mr. Manuel Eisenbarth for his unlimited support and help especially over the thesis time. 8
9 1 INTRODUCTION The purpose of this thesis work is to summarize the mathematical procedure to calculate the bending stiffness of symmetrical and unsymmetrical beams with different cross sections such as I, Rectangular, and Tcrosssections. This paved the way for the summary of the experimental verification by mathematical data processing of the flexural rigidity by 3point, a review on composites and metals as well the comparison between them. Moreover, it is intended to summarize on some examples the theoretical and experimental flexural rigidity and to review international measurement standards for polymer and composite materials, finally, using the CCSM (Composite Compressive Strength Modeler) for deformation analysis of composite materials. 1.1 Problem Definition Structural efficiency is one of the most important character to engineers in the aerospace, boats, car industries and in many other fields. Therefore, a highperformance product made of lightweight materials and yet efficient to withstanding harsh loading conditions is required. The stiffness as a material property is very important in structural engineering as it extents the materials resist deformation in response to applied load. The use of sandwich composites has been considered in this thesis due to the relevance of its stiff light weight structure, which significantly increases the load resistance capacity on one hand without much increase in weight on the other hand. To design a member such as a beam, it is very essential to make sure that it satisfies specific strength, stability, and deflection requirements. Therefore, the bending stiffness analysis plays a major role in choosing materials as it shows how a component behaves under certain loads. 9
10 1.2 Aims and Objectives In order to fulfil the aim of this thesis, the research is conducted aiming to calculating mathematically the flexural rigidity of symmetrical cross sections, verify the experimental results of mathematical data processing of the flexural rigidity by 3point bending, present some examples to illustrate the theoretical and experimental flexural rigidity, review of verification methods for 4point bending, comparing composite materials to metals using some international measurement standards and using composite compressive strength modeler (CCSM) software for modelling of flexural rigidity. 1.3 Method In order to achieve the aim of this thesis and get the theoretical knowledge of the problem, the theory of bending stiffness for different beams and plates have been studied. In the consideration of the bending stiffness analysis of composite material structures, the composite compressive strength modeler (CCSM) and experiments on different materials in the laboratory have been conducted. There are several software packages available for rigidity analysis and deformation tests. In this thesis work, the composite compressive strength modeler (CCSM) software is used for flexural rigidity simulation. 1.4 Background Flexural rigidity is related to bending and nonrigid structures as a force couple that is required to bend a nonrigid structure in one unit of curvature, where force couples also known as pure moments are the forces that rotate a body without translation or acceleration of the center of mass. [1] Since force couples are free vectors in rigid bodies, their effects on a body are independent of the point of application. A couple is known as a combination of two forces, they are equal in magnitude, asymmetrically directed, and displaced by a perpendicular distance or moment. [1] 10
11 1.4.1 Flexural Rigidity Flexural rigidity can be modelled by using different methods. In this scientific discourse, three of the very wellknown methods in the bending stiffness of a profile are treated. The first method can be applied when the modulus is constant, and the cross section is simple then the single formula of second moment of inertia (equation 2, p.12) can be used to obtain the required results of flexural rigidity D. [2] The second method is used when the modulus is constant, and the cross section is not simple but can be however reduced to a simple cross section with a displacement from the neutral axis, in this case the parallel axis theorem can be used effectively by determining the second moment of area or mass moment of inertia of a rigid body about any axis. [3] While the third method which is known as the sandwich beam theory or the Euler Bernoulli beam theory that describes the behavior of a beam, plate, or a shell when calculating the loadcarrying and deflection characteristics of beams. It is used when the profile is not constant in bending modulus, but the profile can be approximated or considered as a layered structure of different materials. [4] The flexural rigidity (D) is defined as EI. In a beam or rod, flexural rigidity varies along the length as a function of (x): Where, x EI dy dx = M(x)dx + C 1 0 (1) [1] E = Young s modulus (Pa) I = second moment of area (m 4 ) y = transverse displacement at x (m) M (x) = bending moment at x (Nm) 11
12 2 THEORY The Euler Bernoulli s Equation and the bending stiffness of a rigid body expresses clearly the flexural rigidity. [1] Euler Bernoulli is known as an engineer of beam theory, which simplifies the linear theory of elasticity. It provides a calculation for the loadcarrying and deflection characteristics of beams and it covers the case for infinitesimal strains and small rotations of a beam which are only subjected to lateral loads. [5] The theory can be extended in a straightforward manner to problems with moderately large rotations by using the von Kármán strains, which provides that the strain remains small. However, in this thesis work the focus is on bending stiffness. [5] Stiffness describes the rigidity of an object, in other words it is the resistance to deformation when a force is applied on it. So, the flexibility of materials is very essential, the more flexible an object is, the less stiff it is. The stiffness of a body is a measure of the resistance offered by an elastic body to deformation. The bending stiffness of a beam is a function of elastic modulus E, the area moment of inertia I of the beam crosssection about the axis of interest, length of the beam and the beam boundary conditions. The bending stiffness of a beam can be analytically derived from the equation of beam deflection when it is applied by a force. [1] 2.1 Second Moment of Area Second moment of area is the property of a cross section. It is normally used to predict the resistance of beams to bending and deflection. The deflection of beams under a certain load doesn t depend only on the load but also on the geometry of the beam s cross section. Beams with a large second moment of area are stiffer than those with a smaller second moment and therefore, they are more resistant to bending. The second moment of area has in other words the meaning of second moment of inertia: [2] I = I 0 + Ad 2 (2) [2] Where, I = second moment of inertia (m 4 ) I0 = second moment of area at centroidal axis (m 4 ) 12
13 A = area (m 2 ) d = distance (m) 2.2 Materials Nowadays, the designing of materials and material properties play a big role in the development of materials. However, there are two main types of materials. The first type is known as structural materials, where the mechanical properties are mainly considered, such as strength, stiffness, and deformation. And the second type is known as functional materials where, the magnetic properties are mainly considered, such as the sound, light, electricity, and heat. [6] Moreover, these materials can be divided into three types depending on the way the atoms or molecules are bonded together. Metallic materials describe the first type, where metal elements are combined with metal bonds, organic polymer materials stand for the second type, where nonmetallic elements are bonded covalently to macromolecular compounds while ceramic materials describe the third type, where nonmetallic elements and metal elements are combined by covalent bonds, ionic bonds, or a mixture of the two bonds. [6] Composite Materials Composite material also known as a multiphase combination material. Composites are formed by combining materials together to form an overall structure with properties that differ from the sum of the individual components. [7] They are generally used for buildings, bridges, and structures due to their benefits such as chemical and corrosion resistance, durable, flexible in design, high flexural modulus to carry demanding loads, high impact strength, high performance at elevated temperature, etc. [7] Composite materials consist of matrix material and reinforcing material as shown in figure 2.1 below, where matrix materials are defined as a continuous phase, which includes metal matrix composite materials, inorganic nonmetallic matrix composite materials as well polymer matrix composites by the different matrix material. Reinforcing material is defined as a dispersed phase which includes usually fibrous materials, such as glass fiber, and organic fiber. [6] 13
14 Figure 2.1 Composite structure [6] Normally the strength of fiber depends on its length and orientation with respect to the stress direction, however, the strength and modulus of fiber are much higher than the matrix material, due its length and accordingly the orientation of stress direction therefore, fibers are the main loadbearing components. However, to firmly bond fibers together, there must be a matrix material with good adhesion properties that can provide a uniformly distributed applied load and transfer the loads to fiber. [6] Composite materials should have at least four characteristics. The composite should be made of a nonhomogeneous material, the components that make up the composite should have different levels of performance, the performance should be the main characteristic of all composites, and the fraction of each component of the composites should be larger than 10 percent of the volume of the composite. [6] Composites versus Metallic Composites and metals have different physical characteristics. For instance, composites are greatly anisotropic which means their properties and values are changeable with direction as well as their strength and stiffness, depending on the orientation of the reinforcing fibers. [8] In addition, composites are lighter in weight, they can tailor the layup for optimum strength and stiffness, improve fatigue life, corrosion resistance, etc. While the metals are isotropic which means their physical properties have the same values in different directions, they are much heavier than composites in weight. Figure 2.2 and table 1 below illustrate an example of some main differences between a composite and a metal. [8] 14
15 Figure 2.2 Steel vs. sandwich [9] Table 1. Composites versus metals under certain conditions. [9] Condition Loadstrain relationship Static Fatigue Transverse properties Mechanical property Fatigue strength Sensitivity to hydrothermal Sensitivity to corrosion Damage growth mechanism Comparative behavior relative to metals More linear strain to failure Greater sensitivity Less sensitivity Weaker Higher Higher Greater Much less Inplane delamination instead of through thickness cracks 2.3 Bending Stiffness of Beams This section covers some concepts about the bending stiffness of symmetrical and unsymmetrical beams with different cross sections, the study of simple bending, and bending of composite beams Theory of Simple Bending with Assumptions Made Simple bending happens at the length of a beam that is subjected to a constant bending moment and when there is no shear force, that is (Q = 0). Which means that the stresses will be arranged along the length of the beam, due to the bending moments only. Therefore, that length of the beam is said to be in pure bending. The assumptions made in the theory of simple bending are known as, the beam is homogeneous and isotropic, the Young s modulus of elasticity in tension and 15
16 compression has the same value, the transverse sections which were plane before bending remain plane after bending, the beam at the beginning of the experiment is straight, and all longitudinal filaments bend into circular arcs with a common center of curvature, the radius of curvature is large compared with the dimensions of the cross section, and each layer of the beam is free to expand or contract, independently of the layer above or below it. [10] However, there are some other tools to use for complicated designs such as a superposition principle or property tool. This tool is used in linear systems for the beams. The superposition principle is one of the most important tools for solving beam loading problems as it allows the simplification of very complicated designs. [10] For the beams that are subjected to several loads of different types the resulting shear force, bending moment, slope and deflection can be found at any location by summing the effects due to each load acting separately to the other loads. The superposition principle is a combination of homogeneity and additivity and satisfies the following equations. [10] Additivity: Homogeneity: F(x 1 + x 2 ) = F(x 1 ) + F(x 2 ) (3) [10] F(ax) = af(x) (4) [10] Simple bending is when a straight bar of homogeneous material is subjected to only a moment at one end and an equal and opposite moment at the other end Bending of Composite Beams A composite beam is made of two or more different materials where these materials are connected rigidly, and the composite behaves like a single piece once it is made. The basic assumption in this case assumes that the plane surface remains plane during bending within the elastic limit [10]. Therefore, the strain remains constant down at the full width of the beam, where the deflection is proportional to the distance from the neutral axis of the beam, in this case the strain can be found easily, and it is equal to (stress/young s Modulus E) [11]. As shown in figure 2.3 below. 16
17 Figure 2.3 Strain [11] The dimensions of the replacement material have the same mechanical properties as the original material, and the overall depth of the transformed section is the same as the original section. Therefore, the resulting strain in any element da of the transformed section must be constant. [11] Strain (ε) = σ (5) [11] E Where, ε = strain (mm/mm) σ = stress (N/m 2 ) E = bending modulus (material property) (Pa) The bending stresses of a composite beam can be calculated using two conditions as follows. [10] 1. The resulted strain on a layer with an equal distance from the neutral axis is the same for both materials. σ 1 E1 = σ 2 E2 σ 1 = σ 2 ( E 1 E 2 ) = mσ 2 (6) [10] 2. The moment of resistance of a composite beam can be determined simply by summing up the individual moments of resistance of the members. M = M 1 + M 2 (7) [10] 17
18 M 1 = σ 1 ( I 1 y ) M 2 = σ 2 ( I 2 y ) M = σ 1 y I 1 + σ 2 y I 2 Where, σ = stress (N/m 2 ) E = bending modulus (material property) (Pa) M = bending moment (Nm) I = moment of inertia (m 4 ) y = distance (m) m = modular ratio, which means in construction the ratio of Young s Moduli of elasticity of the two different materials. (N/m 2 ) Symmetrical Bending The symmetrical bending can be defined as a bending where the bending moments are symmetrical around the neutral axis that passes through the center. Symmetrical bending mainly happens in beams that have symmetrical cross section which can be either single or double layers. [11] The second moment of area which is needed in calculations of bending in beams and also known as the moment of inertia of a shape, it depends on the geometry of objects and it describes how points or particles of an object or an area are distributed about an axis that can be chosen arbitrarily. [11] Examples of Symmetrical Bending One of the examples of symmetrical bending is an Icrosssection beam. Tension and compression loads are applied to the flanges and the body (web) is the core that keeps the facings in place by resisting transverse shear loads. [12] The second moment of area is very high in Isection beam because most of its material is located in the flanges which are placed far from the center of bending (neutral axis), 18
19 and the web has enough material that makes the flanges work together and resist shear and buckling. [12] There are different ways to calculate the bending stiffness of beams. However, for the following shape as an example and since the beam is symmetric from the top to bottom, there is no need to find the centroid of the location. [13] Figure 2.4 Ibeam [13] As it shows from the figure 2.3 above, the I cross section consists of three pieces, instead of treating each piece separately and making separate calculations. It is valuable to treat the whole beam as a rectangle and as a total solid cross section which can be divided into two symmetrical pieces around xaxis and since the centroids of all segments lie on xaxis, there is no need to use the parallel axis theorem. [13] So, the solution for this particular example can be obtained using the following simple moment equation. I x = 1 12 b centerh 3 center The flexural rigidity can be determined from equation 1 page 13. (8) [13] However, in the case of taking all three pieces into consideration, knowing that the beam is symmetric and the center of gravity in the middle then the flexural rigidity D is: [1] D = D i = E(I top + I bottom + I center ) (9) Considering that, [13] I center = 1 12 b 3 centerh center 19
20 And for the bottom and top parts, there is a distance d from the neutral line, so the moment is: [3] I = I center + Ad 2 I top = 1 12 b 3 toph top + b top h top d 2 Where the displacement d is: And the area A is: Since it is symmetric then: d = h center 2 A = b top h top I top = I bottom + h top 2 Another wellknown example of a symmetrical bending is a rectangular cross section beam. The calculation in this case can be done in different ways, one way is by finding the second moment of inertia of the area of a structural section and using the parallel axis theorem. Another common way used in calculations is known as section modulus method. An explanation of both methods is discussed below. [12] 1. Parallel Axis Theorem: In this method a rectangular cross section beam that has a width b and height h is considered as shown in figure 2.4 below. Figure 2.5 Rectangular crosssection Then the area A is: A = b h (10) [12] 20
21 And the moment of inertia I around xaxis that passes through the centroid of the rectangle is: I = 1 12 bh3 And it can be used to calculate the flexural rigidity as follows: [12] D = E I = E 1 12 bh3 When the rotation is around an axis at a distance d from xaxis and is parallel to the centroidal axis as shown in figure 2.6 below. Figure 2.6 Centroidal xaxis Then we use the following parallel axis theorem: [3] I x = I x + Ad 2 2. Section Modulus Method: In this method the crosssection beam is considered to be symmetric from top to bottom, so there is no need to find location centroid. Therefore, the entire rectangle is taken as a total solid cross section and divided into many sections. However, in this thesis work two, four, and six sections are considered below. [13] TwoSection Modulus: In this case a rectangular beam is cut into twosection modulus as in figure below. 21
22 Figure 2.7 Twosections The moment of inertia for each element from top to bottom in this case can be obtained first and then summing up to get the main moment I which can be used to calculate the flexural rigidity as below: For each element top or bottom: [3] Where, I = I 0 + Ad 2 A = b h 2 d = h 4 I 0 = 1 12 b (h 2 ) 3 b = width (m) h = height (m) The moment of inertia for the upper part of the beam is found by substituting A and r into moment equation so we get: I up = 1 12 b (h 2 ) 3 + b ( h 2 ) (h 4 ) 2 I up = 1 96 bh3 + bh And the moment of inertia for the bottom part is determined by substituting the same A and r values into the moment equation again, taking into consideration the negative sign of d, that is (d). So, we get: 22
23 I down = 1 12 b (h 2 ) 3 + b ( h 2 ) ( h 4 ) 2 I down = 1 96 bh3 + bh Then the total moment I is the sum of top and bottom moments: I tot = I up + I down = 2I = bh ( ) 2 = bh 3 ( ) 2 = bh So, the flexural rigidities can be calculated when E, b, h are given and as follows: D = E I tot D = E (bh ) FourSection Modulus: In this module the beam is divided to four sections, the individual moments are calculated in a similar way to the twosection modulus and then the total moment is substituted in the equation of flexural rigidity. The figure 2.8 below illustrates the sections and dimensions used in calculations. Figure 2.8 Foursections For each element top or bottom: [3] I = I 0 + Ad 2 23
24 Where, A = b h 4 That leads to, d = h 8 I 0 = 1 12 b (h 2 ) 3 The first moment I 1 can be obtained by substituting these values into the following equation: I 1 = I 0 + Ad 2 = 1 12 b (h 2 ) 3 + bh 4 (h 8 ) 2 I 1 = bh 3 ( ) = bh 3 ( ) For I 2 an additional distance of ( h ) which is 4 (h) + 8 (h ) is considered in calculations as 8 shown below: I 2 = b (h 4 ) + bh 4 (h 4 + h 2 8 ) = 1 h3 b b h 2 4 (3h 8 ) I 2 = bh 3 ( ) The moments I3 and I4 can be obtained in the same way and then Itotal which is the sum of the moments of all elements is substituted in the flexural rigidity equation 1 page 13. Moreover, the moments related to the thickness t can be calculated in a similar way. The general formula for the moment I in this case is: So, for I 1 with thickness t1 we get: I = 1 12 b(4t)3 = bt (11) [3] 24
25 I 1 = 1 12 bt bt ( t 2 ) 2 And for I 2 we get, I 2 = 1 12 bt bt ( t 2 ) 2 For the first and the second moment I 1/2 we get, I 1/2 = b ( 1 12 t3 + t ( t 2 ) 2 ) 2 I 1/2 = bt 3 ( ) 2 = bt3 ( ) 2 I 1/2 = bt In a similar way the third and the fourth moments are obtained and then we get I 3/4 : I 3/4 = b ( 1 12 t3 + t ( 3 2 t) 2 ) 2 I 3/4 = bt 3 ( ) 2 = 4 + (9 12) bt3 ( ) 2 48 I 3/4 = bt = bt So, I total is: I tot = I i = I 1/2 + I 3/4 = bt3 24 (128) I tot = bt It can be seen from the values obtained for the moments of the outer and the inner layers, that is values of I 1/2 and I 3/4 that the outer layer contributes seven times more to the rigidity than the inner layer, since the ratio of the outer and the inner layer is: = 7 25
26 SixSection Modulus: In this symmetric six section module, the moments for three layers will be considered and calculated and then generalize the results to the other three since the module is symmetric as shown below. Figure 2.9 Sixsections For each element top or bottom: Where, I = I 0 + Ad 2 A = b ( h 6 ) And the three distances are: d 1 = h d 2 = h 6 + h 12 d 3 = h h 12 Applying the general moment equation below: I = 1 12 b (h 6 ) 3 + b h 6 ( h 12 ) 2 (12) [2] 26
27 Then we get I 1 : I 1 = bh 3 ( 1 12 (1 6 ) ( 1 12 ) 2 ) = bh 3 ( ) = bh And for I 2 we get: I 2 = b (h 6 ) + b ( h 2 6 ) (3h 12 ) I 2 = bh 3 ( 1 12 (1 6 ) (1 4 ) 2) = bh 3 ( ) = bh In the same way I 3 : I 3 = 1 12 b ( (h 6 )3 + b ( h 6 ) ( 5 12 h)2 ) I 3 = bh 3 ( 1 12 (1 6 ) ( 5 12 ) 2 ) = bh 3 ( ) = bh The ratios of I 2 and I 1 the outer and the inner layers are: 7 1 = 7 The second outermost contributes seven times more to rigidity than to the innermost. The ratios of I 3 and I 1 the outer and the inner layers are 19 1 = 19 27
28 And the outermost contributes nineteen times more to rigidity than the innermost. From the results and as a conclusion, it can be seen that the outer moments are also dominating in this case by comparing the obtained values of I1, I2, and I3 which gives a clear idea that the rigidity is higher at outer layers, according to the equation of flexural rigidity. It should be mentioned that in a rectangular cross section the contact force and deflections are of great importance, especially when the contact force is directly proportional to the area moment of inertia I of the cross section, where the elastic modulus of the beam material and the beam geometry play a big role in the amount of stress and applied force. So, for instance when the beam is pushed down, there will be an upward restoring force which is equal in magnitude but in opposite direction to the applied force as shown in figure 2.11 below. [14] Figure 2.10 Rectangular beam [15] Figure 2.11 Upward restoring force [15] These forces, deflection, yield, and maximum deflection can be calculated according to the following formulas. Contact Force: F = [ E w t 4 L 3 ] d (13) [14] Deflection at the yield: Y yield = 2 L 2 3 E t σ yield (14) [14] Maximum deflection at load: Y = Fl3 48EI (15) [14] 28
29 Contact force at yield: F yield = [ E w t3 4 L 3 ] d yield (16) [14] = [ E w t3 4 L 3 ] [ 2 L2 3 E t ] σ yield Where, Y = deflection (mm) d = distance (m) F = force (N) σ = stress (N/m 2 ) L = length (m) t = thickness (m) w = b = width (m) I = area moment of inertia (m 4 ) E = bending modulus (material property) (Pa) For known parameters such as dimensions, applied force, and other parameters then the maximum deflection at load for instance can be calculated from equation 19 by using flexural rigidity equation. Which shows the importance of flexural rigidity when studying deflection, contact force at yield, deflection at yield, etc Unsymmetrical Bending In the case of nonsymmetrical section, the neutral axis doesn t pass through the center of the geometrical section. So, the value of y which is the distance of the layer from the neutral axis varies for layers that are located for example at the top and bottom of the section. In order to calculate the bending and since the module is unsymmetrical, the center of gravity of the sections must be found first. [10] The center of gravity (Cg) is defined to be the center to an object s weight distribution, where the gravity force is considered. It is the point where the object is balanced completely, regardless of point of rotation or turning around. Knowing that the neutral axis normally passes through the center of gravity of the section, so by calculating the 29
30 center of gravity of the section, one can find the y values for topmost layer as well for the bottom layer of the section. [10] To more explain the unsymmetrical module, a Tcrosssection example is studied. The top part of the slab is called flange which resists the compressive stress and the part that lies below the slab is called rib which resists the shear stress. [10] Figure 2.12 Tbeam [16] To find the moment, the centroid X and y of a Tsection are calculated first: X = a 1x 1 + a 2 x 2 a 1 + a 2 (17) [16] y = a 1y 1 + a 2 y 2 a 1 +a 2 (18) [16] Where, a1 and a2 are the areas of the flange and rib respectively. The second moment Ixx is: [16] I xx1 = 1 12 W 1H a 1 k 3 2 I xx2 = 1 12 W 2H a 2 k
31 I xx = I xx1 + I xx2 Where, k i = Radius of gyration k 3 = y y 1 To calculate Iyy: [16] k 4 = y y 2 I yy1 = 1 12 W 1H a 1 k 1 2 I yy2 = 1 12 W 2H a 2 k 2 2 I yy = I yy1 + I yy2 Where, k i = Radius of gyration k 1 = x x 1 k 2 = x x 2 So, the flexural rigidity is obtained as in previous sections by substituting the total moment I in the rigidity formula. 2.4 History of Sandwich Structure According to [17]. Delau in England introduced the first sandwich construction, back to Fairbairn The first use of sandwich panels aircraft sandwich was used in World War II. Mainly because of the lack of other materials during the war. The Sandwich Structure theoretically appeared in the 50 s. The use of sandwich structure had some limitation in aircraft industry as honeycomb was mainly used as core material and there were big problems with corrosion due to water absorption, UVRadiation, aging etc. [4]. Figure 2.14 below illustrates the Sandwich Structure efficiency. 31
32 Figure 2.13 Efficiency of sandwich structure [9, p. 256] However, during the early 60 s, there was a production of different cellular plastics which were suitable as core materials. Soft materials were used in the beginning because of their insulation properties such as polystyrene and polyurethane. Later sandwich structure became very useful and flexible concept as harder cellular plastics with higher densities were possible to produce caused by diverse progresses in material production. [17] Nowadays, there is an enormous number of different qualities of cellular plastics that are used as core materials. Sandwich panels became an important composite structure in aerospace applications as well as in high performance automobiles, boats, and wind turbines, because it is an extremely lightweight type of construction that exhibits high stiffness and high strengthtoweight ratios. [4] Sandwich Structure The importance of studying and analyzing these structures is growing as mentioned in the history of sandwich structure. The calculation for flexural rigidity and other quantities can be seen clearly when considering a sandwich structures as they are a suitable example of composites. Sandwich structure consists of two stiff, strong faces separated by a lightweight core and joints (adhesives), which can be seen in figure 2.14 below. [4] 32
33 Figure 2.14 Sandwich structure [18, p. 5] Facing sheets of a typical sandwich structure are mainly thin with a relatively thick lightweight core that separates the two faces in order to increases the moment of inertia. It is for important for engineers or designers of sandwich structures to make the core strong enough to withstand heavy loads and keep their positions. [9] Each component of the sandwich structures has some specific properties that make the sandwich function effectively as a oneunit object. It is preferred by engineers to make the faces of the sandwich structure from some very wellknown metals such as steel, stainless steel, or aluminum due to their stiffness and strength, due to the fact that these materials have some special mechanical properties and they are uncomplicated to use and fabricate. However, in some cases fiber  reinforced plastics are used as face materials as well, because they have good physical properties such as strength. [17] The core has several critical capacities. It must be sufficiently stiff to keep the separation between the faces steady and it must be so rigid in shear to prevent the faces from sliding over each other. The core must be strong in shear to keep the faces cooperating with each other, if the core is weak in shear, the sandwich loses its stiffness. To keep the faces and the core cooperating with each other, the adhesive layer must be added as it enables the transmission of the shear forces between the faces and the core. The adhesive must have the capacity to carry shear and tensile stresses. [4] Flexural Rigidity in Sandwich Beams Since sandwiches are composites and according to their properties, engineers managed to modify and adjust the beam theories so that they can be applied to the sandwich structures and can be used in analyzing and calculating flexural rigidity of sandwiches. [4] 33
34 Figure 2.15 Sandwich beam cross section [4] For beams, the sandwich is slightly different, and it consists of a few different parts where the entire section should be considered when measuring its parts around the centroidal axis. [4] So, the flexural rigidity can be determined as follows: D = Ef ( bt3 6 ) + Ef (btd2) + Ec (bc ) (19) [4] Where, Ef = moduli of elasticity of the faces (index f) Ec = moduli of elasticity of the core (index c) Equation 22 above consists of three terms that calculates flexural rigidity depending on the local flexural rigidity of the faces about their own centroidal axes, bending about the centroidal axis of the entire cross section and the flexural rigidity of the core about its own centroidal axis. [4] When this equation is applied to a sandwich structure and comparing the results to the results obtained earlier for a sixsection modulus found in page 2829, it can be seen that the sandwich is a special case of a sixlayer parallel axis theorem. According to some studies and experiments on sandwich structure with thin faces, engineers and scientist concluded that the amount of flexural rigidity due to faces around their own centroidal axis is very small (less than 1%) compared to the rigidity of the bending of the entire cross section around the centroidal axis, therefore it can be neglected especially when: d t >
35 And the proportion is less than 0.25% at a ratio of: d t > Since the faces are thin, not only the first term can be ignored but in fact experiments showed that the third term of equation 28 is also very small (less than 1%) of the second term which means that it can be ignored as well when: ( E f E c ) ( td2 c 2 ) > 16.7 (20) [4] So, the formula for flexural rigidity D is then reduced to: D = Ef ( btd2 2 ) (21) [4] As a mentioned earlier this is almost the same case as sixsection module and when applying the parallel axis theorem, one would expect the same calculations and results. So, the expectation is that the rigidity at the outer layers contributes with a higher amount of flexural rigidity than the inner layers when considering the entire sandwich structure Deflection of Beams This section deals with beam deflection. Deflection occurs when a specified load is applied to a cross section beam, and the amount of deflection and stress are very important to determine for sandwich structures and beams, for example in case of sandwich, as the core has a relatively low shear modulus, and the beam may deflect a considerable amount due to shear deformations, to neglect the proper consideration of the shear modulus of the core may lead to unconservative prediction of deflections or critical loads. [11] In addition, it is very important to know the limits of deflections for sandwich structure beams to ensure the integrity and stability of a structure or to prevent any attached brittle materials from cracking Therefore, it is essential to determine the modulus and take its effect into account. [19] 35
36 The deflection of beams depends mostly on the modulus of elasticity of the chosen material and must occur within the elastic limit of the material. They are determined using the elastic theory. There is always some additional deflection in the material due to shear, but it is normally so small that it can be neglected. Figure below illustrates the deflection and curvature due to bending. [11] Figure 2.16 Deflection and curvature due to bending [20] There are different types of supports for example supports that resist a force like a pin or a displacement, another supports for instance resist a moment like a fixed end support, resist displacement or a rotation [20]. The following examples illustrate the deflection of a cantilever and a simply supported beam. [21, pp ] Cantilever beam: A cantilever beam is when a beam is attached at only one end and free on the other end as shown in figure below. [21, pp ] Figure 2.17 Cantilever beam [20] The deflection for a cantilever beam at any section in terms of x at free end is given by: And the maximum deflection at the free end is: Y = Fx2 6EI (3L x) (22) 36
37 Y max = FL3 3EI (23) When the load F is concentrated at any point as shown below, then the deflection is: Y = Fx2 (3a x) for 0 < x < a 6EI (24) And the maximum deflection in this case is: Y = Fa2 (3x a) for a < x < L 6EI Y max = Fa2 3EI (3L a) (25) When the load is constant and uniformly distributed (W), then the deflection is: Y = Wx2 24EI (x2 + 6L 2 4Lx) (26) And the maximum deflection in this case is: Y max = WL4 8EI (27) When the load is variable but still uniformly distributed then the deflection is: Y = W 0x 2 120LEI (10L3 10L 2 x + 5Lx 2 x 3 ) (28) Similarly, the maximum deflection in this case is: Y max = W 0L 4 30EI (29) For the couple moment M at the free end of the beam, we have: And maximum is: Y = Mx2 2EI Y max = ML2 2EI (30) (31) 37
38 Where, Y = deflection (mm) x = d = distance (m) F = force (N) L = length (m) I = area moment of inertia (m 4 ) E = bending modulus (material property) (Pa) M = bending moment (Nm) W = distributed load (N/m) Simply supported beam: A simply supported beam has pinned support at one end and a roller support at the other end. In figure 2.17 below represents the pinned end and B the roller end. [21, pp ] Figure 2.18 Simply supported beam [20] The governing equations of this module are very similar to the previous case when it comes to types of loads, location of the loads, etc. A review and brief description of the equations are given and illustrated in figure below. Figure 2.19 Simply supported beam, deflection at center 38
39 Deflection at concentrated load (P = F) at the center is: Y = Fx 12EI [3L2 4 x] for 0 < x < 1 2 (32) [20] And the maximum deflection (δ max = y max ) at the center is: Y max = FL3 48EI (33) [20] Concentrated load F at any point: Y = Fbx 6LEI (L2 x 2 b 2 ) for 0 < x < a (34) Y = Fb 6LEI (L b (x a)3 + (L 2 b 2 )x x 2 ) for a < x < L Maximum deflection at the center: Y max = Fb(L2 b 2 ) 3/2 9 3LEI at x = (L 2 b 2 )/ 3 (35) Y = Fb 48EI (3L2 4b 2 ) at the center if a > b Figure 2.20 Simply supported beam, uniformly distributed load For a uniformly distributed load (ω = W)N/m as shown in figure 2.20 above, then equations are: Y = Wx 24EI (L3 2Lx 2 x 3 ) (36) 39
40 Maximum deflection: Y max = 5WL4 384EI (37) When the load is uniform and variable, then deflection can be expressed as: Y = When the couple moment M is at the right end, then: And the maximum is: Where, Y = deflection (mm) x = d = distance (m) F = force (N) L = length (m) Y max = I = area moment of inertia (m 4 ) E = bending modulus (material property) (Pa) M = bending moment (Nm) b = width (m) W = distributed load (N/m) W 0x 360LEI (7L4 10L 2 x 2 + 3x 4 ) (38) Y = MLx x2 (1 6EI L 2 ) (39) ML2 9 3EI at x = 1/ 3 (40) 40
41 3 METHOD For the practical part and laboratory experiments of this thesis work, the following module, software, and concepts are considered. 1. Composite Compressive Strength Modeler (CCSM) 2. A case of a solid UD lamina 3. Sandwich structure 4. ThreePoint and FourPoint bending 5. Data analysis 3.1 Composite Compressive Strength Modeler (CCSM) According to User s Manual of CCSM modeler, it deals with many different aspects of beams and plates in terms of deflection, flexural rigidity, etc. Some of the main features of this software include classical laminate theory, stressstrain analysis, failure prediction for composite plates, and a very useful userexpandable database to store material and geometrical properties. However, in this thesis work the modeler is used for determining the stiffness and compliance matrices of beams when sufficient information about the beams, lamina, stiffness, etc. are given. [22] In this thesis work when stiffness and compliance matrices are considered using CCSM modeler the flexural rigidity D will be calculated using width (b) and d 11. And in this case, it is: D theory = b d 11 (41) [22] A Solid UD Lamina A lamina is a building block of modern composites laminated structures, a lamina is also known as a ply or a layer and in our case the UD lamina refers to a unidirectional lamina since each lamina may have more than one type of fibers and these fibers may be oriented in different directions, different thickness, fiber orientation angle and matrix material. [22] 41
42 The geometry of a laminate is normally layers that have three planes of material that are symmetric. Therefore, they exhibit orthotropic behavior (having three mutually perpendicular planes of elastic symmetry at each point). When a lamina cut cross these planes of symmetry, they will exhibit the same mechanical properties. Lines which are normal to these planes of material symmetry are called material axes which are designed as 1, 2, and 3 they are also known as principal material directions. Figure 3.1 below illustrate these axes in a UD lamina. [22] Figure 3.1 Principal material axes in a UD lamina [24] When dealing with fibers, matrix and lamina, it should be mentioned that fibers strength and stiffness are significantly larger than that of the matrix, a lamina is stiffest and strongest in longitudinal direction which is the 0degree direction and they are very weak in the 90degree direction because the load must be carried by the much weaker polymeric matrix. A lamina s mechanical properties in any direction lying in the 23 planes are quite similar and therefore, a unidirectional lamina is considered as transversely isotropic. Each layer has approximately the same properties inplane but different properties through the thickness. [23] 3.2 Bending Bend testing also known as flex or flexural testing is commonly performed to measure the flexural strength and modulus of all types of materials and products. The bending of a material or product can be tested using a bending machining tool. [24] 42
43 A universal bending machine consists of a basic machine that can be adjusted and used for a variety of bends. The basic machine consists of a CNCoperated (computer numerically controlled), a work bench and a software for programming and operating. There are three key analysis when performing bend testing which are, the flexural modulus that deals with measuring slope, stressstrain curve, and stiffness of materials, flexural strength which measures the maximum force that a material can resist before it breaks or yields, and yield point of a material, it is a point at which the material can t restore its normal shape after it. [24] ThreePoint & FourPoint Bending Flexural rigidity, modulus of elasticity and other related quantities can be determined when the values of ThreePoint bending are given. The advantage of using threepoint flexural test is the ease of the specimen preparation and testing. Therefore, the threepoint bending will be the module in the practical part of this thesis work. [25] The fourpoint bending flexural test is very similar to the threepoint bending test. The major difference is the addition of a 4 th bearing, which brings a much larger portion of the beam to the maximum stress. This difference needs to be taken into account when studying for example the brittle materials, since it can be used to indicate the flexural strength and crack initiation for instance, in case of asphalt mixtures that are used in road paving, however the fourpoint bending test won t be included in the practical part of this scientific discourse. [26] 43
44 Tables below show some international standard testing methods. Table 2. ASTM standards for threepoint bend. [27] ASTM ASTMC1161 ASTMC1341 ASTMC1684 ASTMC203 ASTMC473 ASTMC598 ASTMC674 ASTMD1184 ASTMD143 ASTMD2344 ASTMD3044 ASTMD349 ASTMD4476 ASTMD7264 ASTMD790 ASTME855 ASTMF1575 ASTMF Standard Test Method Flexural Strength of Advanced Ceramics at Ambient Temperature Flexural Properties of Continuous Fiber Reinforced Advanced Ceramic Composites Flexural Strength of Advanced Ceramics at Ambient TemperatureCylindrical Rod Strength Breaking Load and Flexural Properties of BlockType Thermal Insulation Physical Testing of Gypsum Panel Products Annealing Point and Strain Point of Glass by Beam Bending for Flexural Properties of Ceramic White Ware Materials form Flexural Strength of Adhesive Bonded Laminated Assemblies Small Clear Specimens of Timber for ShortBeam Strength of Polymer Matrix Composite Materials and Their Laminates Shear Modulus of WoodBased Structural Panels Laminated Round Rods Used for Electrical Insulation Flexural Properties of Fiber Reinforced Pultruded Plastic Rods Flexural Properties of Polymer Matrix Composite Materials Flexural Properties of Unreinforced and Reinforced Plastics and Electrical Insulating Materials Bend Testing of Metallic Flat Materials for Spring Applications Involving Static Loading Determining Bending Yield Moment of Nails Components Used in the Surgical Fixation of the Spinal Skeletal System 44
45 Table 3. ASTM standards for fourpoint bend. [27] ASTM ASTMC1161 ASTMC1341 ASTMC1368 ASTMC1576 ASTMC158 ASTMC1674 ASTMC1684 ASTMC393 ASTMC480 ASTMC651 ASTMD6272 ASTMD7249 ASTMD7264 ASTMD790 ASTME855 Standard Test Method Flexural Strength of Advanced Ceramics at Ambient Temperature Flexural Properties of Continuous Fiber Reinforced Advanced Ceramic Composites Determination of Slow Crack Growth Parameters of Advanced Ceramics by Constant StressRate Strength Testing at Ambient Temperature Determination of Slow Crack Growth Parameters of Advanced Ceramics by Constant Stress Flexural Testing (Stress Rupture) at Ambient Temperature Strength of Glass Flexure (Determination of Modulus of Rupture) Flexural Strength of Advanced Ceramics with Engineered Porosity (Honeycomb Cellular Channels) at Ambient Temperatures Flexural Strength of Advanced Ceramics at Ambient TemperatureCylindrical Rod Strength Core Shear Properties of Sandwich Constructions by Beam Flexure Flexure Creep of Sandwich Constructions Flexural Strength of Manufactured Carbon and Graphite Articles Using FourPoint Loading at Room Temperature Flexural Properties of Unreinforced and Reinforced Plastics and Electrical Insulating Materials by FourPoint Facing Properties of Sandwich Constructions by Long Beam Flexure Flexural Properties of Polymer Matrix Composite Materials Flexural Properties of Unreinforced and Reinforced Plastics and Electrical Insulating Materials Bend Testing of Metallic Flat Materials for Spring Applications Involving Static Loading 45
46 4 RESULTS This section deals with the results, graphs, CCSM modeler, experiments, and data analysis in both theoretical and experimental cases as below. 4.1 Bending Test and CCSM Modelling In this section the goal is to make a comparative analysis between theoretical and experimental flexural rigidity D on a solid fiberglass and a sandwich beam with different orientations using the material testing machine under threepoint bending with a uniform constant load and the CCSM modeler for the theoretical part. Figure 4.1 Materials testing machine 46
47 A solid beam of 10 plies and a sandwich beam of 4 plies are used as examples to obtain the theoretical results of stiffness and compliance matrices for zero degree [0º] using the software package CCSM modeler. The CCSM modeler program can be used by entering the obtained geometry of the beam, that is, the required beam dimensions, save ply data in the input and then calculate for elastic properties according to the user s manual. It should be mentioned that for the sake of time saving and ease of use the same lamina properties and thickness can be saved and used for other layers as long as they are of the same material. However, when the lamina is of different material then the reentering data of each lamina along with corresponding properties is required. 1. Theoretical test solid fiberglass (CCSM modeler): The module in this example as mentioned earlier is symmetric and all layers are made of same material (fiberglass). Both theoretical and experimental tests are applied to this module according to the values given in the table below. Table 4. Values for the CCSM Modeler. Property Symbol Unit Width b 25 mm Thickness (unidirection) ta 0.75 mm Longitudinal modulus E GPa Transverse direction E GPA Poisson number Nu 0.3 Shear Modulus G12 2.1GPa Angle 0 47
48 The first step is to enter the above data to the CCSM modeler. Figure 4.2 Solid fiberglass  theoretical The data used in this example are taken from a real lamina tested in the laboratory using a microscope. So, the data are almost exact. After running the software, the following results are obtained, and we are mainly interested in the d11 value that will be used in determining the value of flexural rigidity. Figure 4.3 Solid fiberglass theoretical d 11 48
49 Based on the CCSM modeler the value of d11 and knowing the total thickness of the lamina, that is: b = 25 mm d 11 = So, the theoretical flexural rigidity is: [22] D theory = b(mm) 25 Nmm2 = 1000 = 32 Nmm d 11 (Nm) The flexural rigidity D theory of the 10 layers fiber glass plies is according to the result above is 32 Nmm Experimental test solid fiberglass: This test is performed in the laboratory using material testing machine model M 3503CT available at Arcada laboratory. The same exact solid beam along with the same exact data are used for this experimental test for the sake of comparison between the theoretical and experimental tests and determining the effectiveness and accuracy of CCSM modeler. Figure below shows the linear elasticity and the slope which is of main interest in calculating flexural rigidity Y (Linear) F (N) y = x R² = X Figure 4.4 Solid fiberglass  experimental 49
50 The experimental calculations of flexural rigidity D are as follows: Slope = df dy = k = 48D L 3 (42) [22] Where, L = length between supports k = Slope = N mm Rearranging the equation 50 leads to: D exp = k L3 48 = k (300mm)3 48 D exp = [ N mm ] [mm3 1 ] = Nmm 2 D exp 31 Nmm 2 The relative error is 1 D exp = 1 31 = 1 0,96875, corresponding to 3.1% D theory Theoretical test sandwich beam (number 1): This example is a sandwich beam with four plies and width of 13mm total, with a 1.5mm width for each face and the longitudinal modulus in this example is assumed 15.5 GPa based on the obtained experimental results of this example as shown in figure 4.5 below. 50
51 Figure 4.5 Sandwich beam 1  theoretical After entering the required data and running the simulation, the following results are obtained as shown below. Figure 4.6 Sandwich beam 1 theoretical d 11 In a similar way to the first case, the theoretical flexural rigidity can be calculated as follows: D theory = b(mm) 100 Nmm2 = 1000 = 155 Nmm2 d 11 (Nm)
52 2. Experimental test sandwich beam (number 1): In this laboratory test a sandwich beam made of core cell M80 and the facings made of vinyl ester is used and the other material properties and constants are taken from table 5 page F [N] y = x R² = Figure 4.7 Sandwich beam 1  experimental Applying the flexural rigidity equation again with the obtained slope k, then: D exp = k L3 48 = k (300mm)3 48 D exp = [ N mm ] [mm3 1 ] = Nmm 2 D exp = 153,3 Nmm 2 The relative error is 1 D exp = 1 153,3 = 1 0, , corresponding to 1,1% D theory
53 1. Theoretical test sandwich beam (number 2): The sandwich beam in this test differs from the previous one by angle of orientation, otherwise all the material, data, dimensions are the same. Figure below shows a screenshot of CCSM modeler with entered data. For convenience and suitability, the longitudinal modulus E11 is taken 50 GPa in this test in order to meet the results obtained from the experimental part, since the slope of the linear elasticity gets much smaller in this case due to orientation of the sandwich beam under threepoint bending. Figure 4.8 Sandwich beam 2  theoretical After running CCSM modeler software, then the following results are obtained for compliance matrix d11. Figure 4.9 Sandwich beam 2 theoretical d 11 53
Mechanics of Materials Primer
Mechanics of Materials rimer Notation: A = area (net = with holes, bearing = in contact, etc...) b = total width of material at a horizontal section d = diameter of a hole D = symbol for diameter E = modulus
More informationChapter 4 Deflection and Stiffness
Chapter 4 Deflection and Stiffness Asst. Prof. Dr. Supakit Rooppakhun Chapter Outline Deflection and Stiffness 41 Spring Rates 42 Tension, Compression, and Torsion 43 Deflection Due to Bending 44 Beam
More information[8] Bending and Shear Loading of Beams
[8] Bending and Shear Loading of Beams Page 1 of 28 [8] Bending and Shear Loading of Beams [8.1] Bending of Beams (will not be covered in class) [8.2] Bending Strain and Stress [8.3] Shear in Straight
More informationQUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS
QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State Hooke s law. 3. Define modular ratio,
More informationAERO 214. Lab II. Measurement of elastic moduli using bending of beams and torsion of bars
AERO 214 Lab II. Measurement of elastic moduli using bending of beams and torsion of bars BENDING EXPERIMENT Introduction Flexural properties of materials are of interest to engineers in many different
More informationLecture 15 Strain and stress in beams
Spring, 2019 ME 323 Mechanics of Materials Lecture 15 Strain and stress in beams Reading assignment: 6.1 6.2 News: Instructor: Prof. Marcial Gonzalez Last modified: 1/6/19 9:42:38 PM Beam theory (@ ME
More informationENG2000 Chapter 7 Beams. ENG2000: R.I. Hornsey Beam: 1
ENG2000 Chapter 7 Beams ENG2000: R.I. Hornsey Beam: 1 Overview In this chapter, we consider the stresses and moments present in loaded beams shear stress and bending moment diagrams We will also look at
More informationMembers Subjected to Torsional Loads
Members Subjected to Torsional Loads Torsion of circular shafts Definition of Torsion: Consider a shaft rigidly clamped at one end and twisted at the other end by a torque T = F.d applied in a plane perpendicular
More informationAdvanced Structural Analysis EGF Section Properties and Bending
Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear
More informationME Final Exam. PROBLEM NO. 4 Part A (2 points max.) M (x) y. z (neutral axis) beam crosssec+on. 20 kip ft. 0.2 ft. 10 ft. 0.1 ft.
ME 323  Final Exam Name December 15, 2015 Instructor (circle) PROEM NO. 4 Part A (2 points max.) Krousgrill 11:30AM12:20PM Ghosh 2:303:20PM Gonzalez 12:301:20PM Zhao 4:305:20PM M (x) y 20 kip ft 0.2
More informationSTRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS
1 UNIT I STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define: Stress When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The
More informationStress Analysis Lecture 4 ME 276 Spring Dr./ Ahmed Mohamed Nagib Elmekawy
Stress Analysis Lecture 4 ME 76 Spring 017018 Dr./ Ahmed Mohamed Nagib Elmekawy Shear and Moment Diagrams Beam Sign Convention The positive directions are as follows: The internal shear force causes a
More informationPERIYAR CENTENARY POLYTECHNIC COLLEGE PERIYAR NAGAR  VALLAM THANJAVUR. DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK
PERIYAR CENTENARY POLYTECHNIC COLLEGE PERIYAR NAGAR  VALLAM  613 403  THANJAVUR. DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Sub : Strength of Materials Year / Sem: II / III Sub Code : MEB 310
More information: APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4021 COURSE CATEGORY : A PERIODS/ WEEK : 5 PERIODS/ SEMESTER : 75 CREDIT : 5 TIME SCHEDULE
COURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4021 COURSE CATEGORY : A PERIODS/ WEEK : 5 PERIODS/ SEMESTER : 75 CREDIT : 5 TIME SCHEDULE MODULE TOPIC PERIODS 1 Simple stresses
More informationProperties of Sections
ARCH 314 Structures I Test Primer Questions Dr.Ing. Peter von Buelow Properties of Sections 1. Select all that apply to the characteristics of the Center of Gravity: A) 1. The point about which the body
More informationQUESTION BANK DEPARTMENT: CIVIL SEMESTER: III SUBJECT CODE: CE2201 SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A
DEPARTMENT: CIVIL SUBJECT CODE: CE2201 QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State
More informationCOURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4017 COURSE CATEGORY : A PERIODS/WEEK : 6 PERIODS/ SEMESTER : 108 CREDITS : 5
COURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4017 COURSE CATEGORY : A PERIODS/WEEK : 6 PERIODS/ SEMESTER : 108 CREDITS : 5 TIME SCHEDULE MODULE TOPICS PERIODS 1 Simple stresses
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationPURE BENDING. If a simply supported beam carries two point loads of 10 kn as shown in the following figure, pure bending occurs at segment BC.
BENDING STRESS The effect of a bending moment applied to a crosssection of a beam is to induce a state of stress across that section. These stresses are known as bending stresses and they act normally
More informationUNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation.
UNIT 1 STRESS STRAIN AND DEFORMATION OF SOLIDS, STATES OF STRESS 1. Define stress. When an external force acts on a body, it undergoes deformation. At the same time the body resists deformation. The magnitude
More informationDownloaded from Downloaded from / 1
PURWANCHAL UNIVERSITY III SEMESTER FINAL EXAMINATION2002 LEVEL : B. E. (Civil) SUBJECT: BEG256CI, Strength of Material Full Marks: 80 TIME: 03:00 hrs Pass marks: 32 Candidates are required to give their
More informationSERVICEABILITY OF BEAMS AND ONEWAY SLABS
CHAPTER REINFORCED CONCRETE Reinforced Concrete Design A Fundamental Approach  Fifth Edition Fifth Edition SERVICEABILITY OF BEAMS AND ONEWAY SLABS A. J. Clark School of Engineering Department of Civil
More informationStructural Dynamics Lecture Eleven: Dynamic Response of MDOF Systems: (Chapter 11) By: H. Ahmadian
Structural Dynamics Lecture Eleven: Dynamic Response of MDOF Systems: (Chapter 11) By: H. Ahmadian ahmadian@iust.ac.ir Dynamic Response of MDOF Systems: ModeSuperposition Method ModeSuperposition Method:
More informationMATERIALS. Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle?
MATERIALS Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: A. Composition
More informationSymmetric Bending of Beams
Symmetric Bending of Beams beam is any long structural member on which loads act perpendicular to the longitudinal axis. Learning objectives Understand the theory, its limitations and its applications
More informationPES Institute of Technology
PES Institute of Technology Bangalore south campus, Bangalore5460100 Department of Mechanical Engineering Faculty name : Madhu M Date: 29/06/2012 SEM : 3 rd A SEC Subject : MECHANICS OF MATERIALS Subject
More informationPurpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on Exam 3.
ES230 STRENGTH OF MTERILS Exam 3 Study Guide Exam 3: Wednesday, March 8 th inclass Updated 3/3/17 Purpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on
More informationJohns Hopkins University What is Engineering? M. Karweit MATERIALS
Why do things break? Why are some materials stronger than others? Why is steel tough? Why is glass brittle? What is toughness? strength? brittleness? Elemental material atoms: MATERIALS A. Composition
More informationCOURSE TITLE : THEORY OF STRUCTURES I COURSE CODE : 3013 COURSE CATEGORY : B PERIODS/WEEK : 6 PERIODS/SEMESTER: 90 CREDITS : 6
COURSE TITLE : THEORY OF STRUCTURES I COURSE CODE : 0 COURSE CATEGORY : B PERIODS/WEEK : 6 PERIODS/SEMESTER: 90 CREDITS : 6 TIME SCHEDULE Module Topics Period Moment of forces Support reactions Centre
More informationCHAPTER 6 BENDING Part 1
Ishik University / Sulaimani Civil Engineering Department Mechanics of Materials CE 211 CHAPTER 6 BENDING Part 11 CHAPTER 6 Bending Outlines of this chapter: 6.1. Chapter Objectives 6.2. Shear and
More informationMECHANICS OF MATERIALS. Prepared by Engr. John Paul Timola
MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationComputational Analysis for Composites
Computational Analysis for Composites Professor Johann Sienz and Dr. Tony Murmu Swansea University July, 011 The topics covered include: OUTLINE Overview of composites and their applications Micromechanics
More informationNORMAL STRESS. The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts.
NORMAL STRESS The simplest form of stress is normal stress/direct stress, which is the stress perpendicular to the surface on which it acts. σ = force/area = P/A where σ = the normal stress P = the centric
More informationHomework No. 1 MAE/CE 459/559 John A. Gilbert, Ph.D. Fall 2004
Homework No. 1 MAE/CE 459/559 John A. Gilbert, Ph.D. 1. A beam is loaded as shown. The dimensions of the cross section appear in the insert. the figure. Draw a complete free body diagram showing an equivalent
More informationDEPARTMENT OF CIVIL ENGINEERING
KINGS COLLEGE OF ENGINEERING DEPARTMENT OF CIVIL ENGINEERING SUBJECT: CE 2252 STRENGTH OF MATERIALS UNIT: I ENERGY METHODS 1. Define: Strain Energy When an elastic body is under the action of external
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More information9 MECHANICAL PROPERTIES OF SOLIDS
9 MECHANICAL PROPERTIES OF SOLIDS Deforming force Deforming force is the force which changes the shape or size of a body. Restoring force Restoring force is the internal force developed inside the body
More informationFlexural properties of polymers
A2 _EN BUDAPEST UNIVERSITY OF TECHNOLOGY AND ECONOMICS FACULTY OF MECHANICAL ENGINEERING DEPARTMENT OF POLYMER ENGINEERING Flexural properties of polymers BENDING TEST OF CHECK THE VALIDITY OF NOTE ON
More informationConsider an elastic spring as shown in the Fig.2.4. When the spring is slowly
.3 Strain Energy Consider an elastic spring as shown in the Fig..4. When the spring is slowly pulled, it deflects by a small amount u 1. When the load is removed from the spring, it goes back to the original
More informationMechanics of Materials II. Chapter III. A review of the fundamental formulation of stress, strain, and deflection
Mechanics of Materials II Chapter III A review of the fundamental formulation of stress, strain, and deflection Outline Introduction Assumtions and limitations Axial loading Torsion of circular shafts
More informationUNIVERSITY OF BOLTON SCHOOL OF ENGINEERING. BEng (HONS) CIVIL ENGINEERING SEMESTER 1 EXAMINATION 2016/2017 MATHEMATICS & STRUCTURAL ANALYSIS
TW21 UNIVERSITY OF BOLTON SCHOOL OF ENGINEERING BEng (HONS) CIVIL ENGINEERING SEMESTER 1 EXAMINATION 2016/2017 MATHEMATICS & STRUCTURAL ANALYSIS MODULE NO: CIE4011 Date: Wednesday 11 th January 2017 Time:
More informationHigh Tech High Top Hat Technicians. An Introduction to Solid Mechanics. Is that supposed to bend there?
High Tech High Top Hat Technicians An Introduction to Solid Mechanics Or Is that supposed to bend there? Why don't we fall through the floor? The power of any Spring is in the same proportion with the
More information7 TRANSVERSE SHEAR transverse shear stress longitudinal shear stresses
7 TRANSVERSE SHEAR Before we develop a relationship that describes the shearstress distribution over the cross section of a beam, we will make some preliminary remarks regarding the way shear acts within
More informationUnit III Theory of columns. Dr.P.Venkateswara Rao, Associate Professor, Dept. of Civil Engg., SVCE, Sriperumbudir
Unit III Theory of columns 1 Unit III Theory of Columns References: Punmia B.C.,"Theory of Structures" (SMTS) Vol II, Laxmi Publishing Pvt Ltd, New Delhi 2004. Rattan.S.S., "Strength of Materials", Tata
More information6. Bending CHAPTER OBJECTIVES
CHAPTER OBJECTIVES Determine stress in members caused by bending Discuss how to establish shear and moment diagrams for a beam or shaft Determine largest shear and moment in a member, and specify where
More informationMechanics of Structure
S.Y. Diploma : Sem. III [CE/CS/CR/CV] Mechanics of Structure Time: Hrs.] Prelim Question Paper Solution [Marks : 70 Q.1(a) Attempt any SIX of the following. [1] Q.1(a) Define moment of Inertia. State MI
More informationCE6306 STRENGTH OF MATERIALS TWO MARK QUESTIONS WITH ANSWERS ACADEMIC YEAR
CE6306 STRENGTH OF MATERIALS TWO MARK QUESTIONS WITH ANSWERS ACADEMIC YEAR 20142015 UNIT  1 STRESS, STRAIN AND DEFORMATION OF SOLIDS PART A 1. Define tensile stress and tensile strain. The stress induced
More informationCIVIL DEPARTMENT MECHANICS OF STRUCTURES ASSIGNMENT NO 1. Brach: CE YEAR:
MECHANICS OF STRUCTURES ASSIGNMENT NO 1 SEMESTER: V 1) Find the least moment of Inertia about the centroidal axes XX and YY of an unequal angle section 125 mm 75 mm 10 mm as shown in figure 2) Determine
More informationHow materials work. Compression Tension Bending Torsion
Materials How materials work Compression Tension Bending Torsion Elemental material atoms: A. Composition a) Nucleus: protons (+), neutrons (0) b) Electrons () B. Neutral charge, i.e., # electrons = #
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationMechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces
Mechanical Behavior of Circular Composite Springs with Extended Flat Contact Surfaces PingCheung Tse epartment of Mechanical Engineering, The Hong Kong Polytechnic University, Hunghom, Kowloon, Hong Kong
More informationCHAPTER 4: BENDING OF BEAMS
(74) CHAPTER 4: BENDING OF BEAMS This chapter will be devoted to the analysis of prismatic members subjected to equal and opposite couples M and M' acting in the same longitudinal plane. Such members are
More informationChapter 6: CrossSectional Properties of Structural Members
Chapter 6: CrossSectional Properties of Structural Members Introduction Beam design requires the knowledge of the following. Material strengths (allowable stresses) Critical shear and moment values Cross
More informationR13. II B. Tech I Semester Regular Examinations, Jan MECHANICS OF SOLIDS (Com. to ME, AME, AE, MTE) PARTA
SET  1 II B. Tech I Semester Regular Examinations, Jan  2015 MECHANICS OF SOLIDS (Com. to ME, AME, AE, MTE) Time: 3 hours Max. Marks: 70 Note: 1. Question Paper consists of two parts (PartA and PartB)
More informationSub. Code:
Important Instructions to examiners: ) The answers should be examined by key words and not as wordtoword as given in the model answer scheme. ) The model answer and the answer written by candidate may
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationD : SOLID MECHANICS. Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown.
D : SOLID MECHANICS Q. 1 Q. 9 carry one mark each. Q.1 Find the force (in kn) in the member BH of the truss shown. Q.2 Consider the forces of magnitude F acting on the sides of the regular hexagon having
More informationGATE SOLUTIONS E N G I N E E R I N G
GATE SOLUTIONS C I V I L E N G I N E E R I N G From (1987018) Office : F16, (Lower Basement), Katwaria Sarai, New Delhi110016 Phone : 01165064 Mobile : 81309090, 9711853908 Email: info@iesmasterpublications.com,
More informationTABLE OF CONTENTS. Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA
Mechanics of Composite Materials, Second Edition Autar K Kaw University of South Florida, Tampa, USA TABLE OF CONTENTS 1. INTRODUCTION TO COMPOSITE MATERIALS 1.1 Introduction... 1.2 Classification... 1.2.1
More informationENG1001 Engineering Design 1
ENG1001 Engineering Design 1 Structure & Loads Determine forces that act on structures causing it to deform, bend, and stretch Forces push/pull on objects Structures are loaded by: > Dead loads permanent
More informationName :. Roll No. :... Invigilator s Signature :.. CS/B.TECH (CENEW)/SEM3/CE301/ SOLID MECHANICS
Name :. Roll No. :..... Invigilator s Signature :.. 2011 SOLID MECHANICS Time Allotted : 3 Hours Full Marks : 70 The figures in the margin indicate full marks. Candidates are required to give their answers
More informationMechanical Engineering Ph.D. Preliminary Qualifying Examination Solid Mechanics February 25, 2002
student personal identification (ID) number on each sheet. Do not write your name on any sheet. #1. A homogeneous, isotropic, linear elastic bar has rectangular cross sectional area A, modulus of elasticity
More informationMechanics in Energy Resources Engineering  Chapter 5 Stresses in Beams (Basic topics)
Week 7, 14 March Mechanics in Energy Resources Engineering  Chapter 5 Stresses in Beams (Basic topics) KiBok Min, PhD Assistant Professor Energy Resources Engineering i Seoul National University Shear
More informationMECE 3321: Mechanics of Solids Chapter 6
MECE 3321: Mechanics of Solids Chapter 6 Samantha Ramirez Beams Beams are long straight members that carry loads perpendicular to their longitudinal axis Beams are classified by the way they are supported
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More informationCHAPTER OBJECTIVES Use various methods to determine the deflection and slope at specific pts on beams and shafts: 2. Discontinuity functions
1. Deflections of Beams and Shafts CHAPTER OBJECTIVES Use various methods to determine the deflection and slope at specific pts on beams and shafts: 1. Integration method. Discontinuity functions 3. Method
More informationSTRENGTH OF MATERIALSI. Unit1. Simple stresses and strains
STRENGTH OF MATERIALSI Unit1 Simple stresses and strains 1. What is the Principle of surveying 2. Define Magnetic, True & Arbitrary Meridians. 3. Mention different types of chains 4. Differentiate between
More informationSRI CHANDRASEKHARENDRA SARASWATHI VISWA MAHAVIDHYALAYA
SRI CHANDRASEKHARENDRA SARASWATHI VISWA MAHAVIDHYALAYA (Declared as Deemedtobe University under Section 3 of the UGC Act, 1956, Vide notification No.F.9.9/92U3 dated 26 th May 1993 of the Govt. of
More information(48) CHAPTER 3: TORSION
(48) CHAPTER 3: TORSION Introduction: In this chapter structural members and machine parts that are in torsion will be considered. More specifically, you will analyze the stresses and strains in members
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More information7.6 Stress in symmetrical elastic beam transmitting both shear force and bending moment
7.6 Stress in symmetrical elastic beam transmitting both shear force and bending moment à It is more difficult to obtain an exact solution to this problem since the presence of the shear force means that
More informationChapter 3. Load and Stress Analysis
Chapter 3 Load and Stress Analysis 2 Shear Force and Bending Moments in Beams Internal shear force V & bending moment M must ensure equilibrium Fig. 3 2 Sign Conventions for Bending and Shear Fig. 3 3
More informationPresented By: EAS 6939 Aerospace Structural Composites
A Beam Theory for Laminated Composites and Application to Torsion Problems Dr. BhavaniV. Sankar Presented By: Sameer Luthra EAS 6939 Aerospace Structural Composites 1 Introduction Composite beams have
More informationOptimum Height of Plate Stiffener under Pressure Effect
The st Regional Conference of Eng. Sci. NUCEJ Spatial ISSUE vol., No.3, 8 pp 459468 Optimum Height of Plate Stiffener under Pressure Effect Mazin Victor Yousif M.Sc Production Engineering University of
More informationInfluence of residual stresses in the structural behavior of. tubular columns and arches. Nuno Rocha Cima Gomes
October 2014 Influence of residual stresses in the structural behavior of Abstract tubular columns and arches Nuno Rocha Cima Gomes Instituto Superior Técnico, Universidade de Lisboa, Portugal Contact:
More informationPart 1 is to be completed without notes, beam tables or a calculator. DO NOT turn Part 2 over until you have completed and turned in Part 1.
NAME CM 3505 Fall 06 Test 2 Part 1 is to be completed without notes, beam tables or a calculator. Part 2 is to be completed after turning in Part 1. DO NOT turn Part 2 over until you have completed and
More informationCHAPTER 5. Beam Theory
CHPTER 5. Beam Theory SangJoon Shin School of Mechanical and erospace Engineering Seoul National University ctive eroelasticity and Rotorcraft Lab. 5. The EulerBernoulli assumptions One of its dimensions
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationFLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR DEFORMABLE PLATE THEORY
AsiaPacific Conference on FRP in Structures (APFIS 2007) S.T. Smith (ed) 2007 International Institute for FRP in Construction FLEXURAL RESPONSE OF FIBER RENFORCED PLASTIC DECKS USING HIGHERORDER SHEAR
More informationKINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK. Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV
KINGS COLLEGE OF ENGINEERING DEPARTMENT OF MECHANICAL ENGINEERING QUESTION BANK Subject code/name: ME2254/STRENGTH OF MATERIALS Year/Sem:II / IV UNIT I STRESS, STRAIN DEFORMATION OF SOLIDS PART A (2 MARKS)
More informationBEAM DEFLECTION THE ELASTIC CURVE
BEAM DEFLECTION Samantha Ramirez THE ELASTIC CURVE The deflection diagram of the longitudinal axis that passes through the centroid of each crosssectional area of a beam. Supports that apply a moment
More informationMechanics of Solids notes
Mechanics of Solids notes 1 UNIT II Pure Bending Loading restrictions: As we are aware of the fact internal reactions developed on any crosssection of a beam may consists of a resultant normal force,
More informationCHAPTER 4. Stresses in Beams
CHAPTER 4 Stresses in Beams Problem 1. A rolled steel joint (RSJ) of section has top and bottom flanges 150 mm 5 mm and web of size 00 mm 1 mm. t is used as a simply supported beam over a span of 4 m
More information2012 MECHANICS OF SOLIDS
R10 SET  1 II B.Tech II Semester, Regular Examinations, April 2012 MECHANICS OF SOLIDS (Com. to ME, AME, MM) Time: 3 hours Max. Marks: 75 Answer any FIVE Questions All Questions carry Equal Marks ~~~~~~~~~~~~~~~~~~~~~~
More information3 Hours/100 Marks Seat No.
*17304* 17304 14115 3 Hours/100 Marks Seat No. Instructions : (1) All questions are compulsory. (2) Illustrate your answers with neat sketches wherever necessary. (3) Figures to the right indicate full
More informationFLEXIBILITY METHOD FOR INDETERMINATE FRAMES
UNIT  I FLEXIBILITY METHOD FOR INDETERMINATE FRAMES 1. What is meant by indeterminate structures? Structures that do not satisfy the conditions of equilibrium are called indeterminate structure. These
More informationUNIT III DEFLECTION OF BEAMS 1. What are the methods for finding out the slope and deflection at a section? The important methods used for finding out the slope and deflection at a section in a loaded
More informationPDDC 1 st Semester Civil Engineering Department Assignments of Mechanics of Solids [ ] Introduction, Fundamentals of Statics
Page1 PDDC 1 st Semester Civil Engineering Department Assignments of Mechanics of Solids [2910601] Introduction, Fundamentals of Statics 1. Differentiate between Scalar and Vector quantity. Write S.I.
More informationBending Load & Calibration Module
Bending Load & Calibration Module Objectives After completing this module, students shall be able to: 1) Conduct laboratory work to validate beam bending stress equations. 2) Develop an understanding of
More informationStresses in Curved Beam
Stresses in Curved Beam Consider a curved beam subjected to bending moment M b as shown in the figure. The distribution of stress in curved flexural member is determined by using the following assumptions:
More informationStrength of Materials Prof. Dr. Suraj Prakash Harsha Mechanical and Industrial Engineering Department Indian Institute of Technology, Roorkee
Strength of Materials Prof. Dr. Suraj Prakash Harsha Mechanical and Industrial Engineering Department Indian Institute of Technology, Roorkee Lecture  28 Hi, this is Dr. S. P. Harsha from Mechanical and
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More information